| ||Format||Pages||Price|| |
|4||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$48.00||  ADD TO CART|
This practice covers procedures that can be followed to safeguard against the possible embrittlement of steel hot-dip galvanized after fabrication, and outlines test procedures for detecting embrittlement. Conditions of fabrication may induce a susceptibility to embrittlement in certain steels that can be accelerated by galvanizing. Open-hearth, basic-oxygen, and electric-furnace steels shall be used for galvanizing. Other materials that can be galvanized include continuous cast slabs, steel or iron castings, and wrought iron. The material shall undergo cold working and thermal treatment. Embrittlement of steel shapes, steel castings, threaded articles, and hardware items shall be tested using a bend test , a universal testing machine, or by means of a press with the load applied slowly, until fracture of the galvanized test specimen occurs.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This practice covers procedures that can be followed to safeguard against the possible embrittlement of steel hot-dip galvanized after fabrication, and outlines test procedures for detecting embrittlement. Conditions of fabrication may induce a susceptibility to embrittlement in certain steels that can be accelerated by galvanizing. Embrittlement is not a common occurrence, however, and this discussion does not imply that galvanizing increases embrittlement where good fabricating and galvanizing procedures are employed. Where history has shown that for specific steels, processes and galvanizing procedures have been satisfactory, this history will serve as an indication that no embrittlement problem is to be expected for those steels, processes, and galvanizing procedures.
1.2 This practice is applicable in either inch-pounds or SI units. Inch-pounds and SI units are not necessarily exact equivalents. Within the text of this practice and where appropriate, SI units are shown in brackets.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.4 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
F606 Test Methods for Determining the Mechanical Properties of Externally and Internally Threaded Fasteners, Washers, and Rivets (Metric) F0606_F0606M
ICS Number Code 77.140.10 (Heat-treatable steels)
UNSPSC Code 30103600(Structural products); 11101704(Steel)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM A143 / A143M-07(2020), Standard Practice for Safeguarding Against Embrittlement of Hot-Dip Galvanized Structural Steel Products and Procedure for Detecting Embrittlement, ASTM International, West Conshohocken, PA, 2020, www.astm.orgBack to Top